N A N O E X P R E S S
Photovoltaic properties of PSi impregnated
, Laura Manca1
, Susanna Setzu1
and Alessandro Pezzella2
A bulk heterojunction of porous silicon and eumelanin, where the columnar pores of porous silicon are filled with eumelanin, is proposed as a new organic-inorganic hybrid material for photovoltaic applications. The addition of eumelanin, whose absorption in the near infrared region is significantly higher than porous silicon, should greatly enhance the light absorption capabilities of the empty porous silicon matrix, which are very low in the low energy side of the visible spectral range (from about 600 nm downwards). The experimental results show that indeed the photocarrier collection efficiency at longer wavelengths in eumelanin-impregnated samples is clearly higher with respect to empty porous silicon matrices.
Keywords:Organic-inorganic interface, Hybrid material, Bulk heterojunction, Eumelanin, Porous silicon, Photoconversion, 5,6-dihydroxyindole
PACS: 88.40.fh, 88.40.jj
The relevance of solar power in the renewable energy field is constantly increasing due to its ready availability and to the fact that the available amount exceeds by sev-eral orders of magnitude the needs of the human race. The search for new materials with better performances than standard Si-based solar cells is also constantly in-creasing. Organic materials  emerged as a very attract-ive solution for this scope, their lower efficiencies with respect to inorganic materials being compensated by lower fabrication costs and higher flexibility. Hybrid materials have also been investigated as a way to com-bine the low production costs of organic materials with the high efficiency of inorganic materials [2-8].
Among the adopted strategies for new materials, inter-face geometry often plays a major role in the collection of photogenerated carriers, and bulk heterojunctions [3,9-12] - intimately mixing the two junction materials
while keeping them separate in a ‘fractal like’
high-surface interface - are a very promising design for solar cells. This concept was introduced in the mid 1990s for
organic solar cells [5,13-15] to shorten the exciton travel distance from the photon absorption site towards the charge-separating interface and then both to reduce the spontaneous recombination and to increase the collec-tion efficiency. The very large interfacial area available for charge separation processes also increases the carrier collection efficiency.
We investigate here a new hybrid material for photovol-taic applications composed byn-type porous silicon (PSi) and eumelanin, a natural pigment featuring relatively high electrical conductivity  and believed to rely mainly on proton-based conduction [16-18]. Porous Si is a large spe-cific area material, whose properties depend on Si sub-strate doping and on fabrication parameters . Its application span ranges from biosensor  to drug deliv-ery  and optoelectronics . In the photovoltaic field, PSi has been considered up to now mainly as an antire-flection coating for crystalline Si , and there are very few studies about its photovoltaic properties [23,24]. Por-ous Si-organic hybrids have recently been considered , but literature reports are mainly on amorphous  or crystalline [27,28] Si. An exception are the interesting results by Nahor et al.  reporting a study of a PSi-organic hybrid material realized using conjugate polymers for solar cells, which highlight the potential of PSi-based bulk heterojunctions.
* Correspondence:email@example.com 1
Dipartimento di Fisica, Cittadella Universitaria di Monserrato, Università degli Studi di Cagliari, S.P. 8 km 0.7, Monserrato (Ca) 09042, Italy
Full list of author information is available at the end of the article
Melanins are a class of natural pigments responsible for the colorations of human skin and hair  in the range from light, yellow-reddish (pheomelanins) and dark, brownish black (eumelanins). Their unique status among natural pigments is due to their socioeconomic and biomedical relevance, encompassing racial tation, skin photoprotection, sun tanning, and pigmen-tary disorders. Moreover, they display a quite unusual set of physicochemical properties such as broadband mono-tonic absorption in the ultraviolet-visible .
These features have suggested the possible use of syn-thetic (artificial) eumelanins in the development of a new generation of bioinspired electrically active devices [30-32]. More recently, eumelanin biopolymers have also been proposed for optoelectronic and photovoltaic appli-cations [33,34]. Due to their wide absorbance covering the whole visible light spectrum, eumelanins behave as very efficient photoreceptors .
As a part of a large project aimed to assess the scope of melanins and melanin-like materials for the develop-ment of novel hybrid functional architectures [35,36], we
investigate here ‘5,6-dihydroxyindole-melanin
immobi-lized PSi’ as a prototypal device for the generation of white light-induced photocurrent.
Methods Porous silicon
PSi samples were prepared by electrochemical etch in the dark of (100)-oriented, phosphorous doped, n+-type monocrystalline Si wafers from Siltronix (Archamps Technopole, Archamps, France) using the procedure described in . The resistivity of the wafers is in the 0.007 to 0.003 ohm/cm range. The constant current etching process [38,39] has been performed in a
polyvi-nylchloride electrochemical cell using HF:H2O:ethanol
solution in 15:15:70 percent, respectively. The potential source was a PARSTAT 2273 potentiostat from Prince-ton Applied Research (Oak Ridge, TN, USA). The vari-ous components of the fabrication cell are schematically shown in Figure 1. The silicon substrate acts as the working electrode and a platinum wire or grid is used as a counter electrode.
All samples considered have a nominal 5μm thickness. The relation between the samples' thickness and their re-spective fabrication time has been studied by means of scanning electron microscopy (SEM). In Figure 2 we show an example of thickness measurement performed on a 29μm-thick PSi sample. The scale is shown at the bottom of the image. The porous layer (comprised between the two orange lines) and the bulk Si substrate are indicated, together with the measured thickness value. The thickness measurements proved to be fully reproducible for any
thickness below or equal to 29 μm (the thickest sample
tested) and directly proportional to the formation time.
The samples' porosity, measured by gravimetry, was 55 % (empty/full ratio) for all samples. A few samples have been electrochemically oxidized, in the same cell used for the formation process, using a 0.1 M aqueous solution of KNO3 and a constant current I=−5 mA. The optical
re-flectivity measurements were performed using a PerkinEl-mer (Perkin ElPerkinEl-mer Italia SpA, Monza (MI), Italy) Lambda 950 spectrometer equipped with the Universal Reflectance Accessory using an incidence angle of 8°.
Eumelanin formation starts from a tyrosinase-catalyzed oxidation of tyrosine (Figure 3) in a multistep process up
HF Solution Pt electrode
Figure 1Schematic of PSi fabrication equipment.The working electrode is the crystalline Si wafer.
to 5,6-dihydroxyindole (DHI) and 5,6 dihydroxyindole-2-carboxylic acid. Oxidative polymerization of these indoles then gives rise to the black-brown variety of melanin bio-polymer: the eumelanin .
In our experiments, DHI  and synthetic eumelanin  were prepared according to the literature: a solution of DHI (50 mmol) in phosphate buffer, 0.1 M, pH 7.4, (10 ml) was treated with tyrosinase (400 units) under a stream of oxygen for 4 h at 25 °C, then acidified to pH 4.5 and washed first with distilled water and then in methanol/water 7/3.
Eumelanin immobilization on porous Si was obtained by treating the substrates with the appropriate solution/sus-pension of DHI or synthetic melanin: methanol, methanol/ water, or methanol/phosphate buffer pH 7.0 were used as liquid phase. The substrates were processed with three cycles, 5 min each, in ultrasound bath, followed by 4 h oxygen exposition. When suitable, tyrosinase was also added to the mixture to promote oxidation process.
Photocurrent measuring procedure
Electrical contacts were realized by deposition of gold spots on top of the empty and impregnated porous layers by sputtering using an Emitech K450 sputter coater (Quorum Technologies Ltd, East Grinstead, West Sussex, UK). On each sample, four contacts were rea-lized to test the reproducibility of the procedure.
The samples' photoconductivity was tested using a PM8 Analytical prober and a Keithley multimeter (Keithley Instruments Inc., Cleveland, OH, USA). The light source was a tungsten-halogen lamp, whose spec-tral range at the output of the optical system was in the 400 to 850 nm interval. The active external surface of the samples involved in the photocurrent generation is estimated of the order of a squared millimeter.
Results and discussion
Different approaches for the immobilization of eumela-nin in the porous matrix have been explored, including treatment of the porous Si with preformed synthetic
eumelanin and in situ-induced oxidative polymerization
To gain insight into the mode of coupling (Figure 3) of DHI during polymer buildup in this procedure, which is important to match the basic structural features of the immobilized DHI-derived polymer [30,32] and to valid-ate the procedure, mother liquors were collected and the reaction was stopped in the early stages by the addition of sodium dithionite to reduce the oxidized species. The
crude oligomer-containing mixture was acetylated
according to an established protocol  and examined by thin layer chromatography (TLC). This treatment of the mixture allowed the isolation of two main eumelanin oligomer intermediates, which were identified as the acetylated 2,7′- and 2,4′-biindolyls.
The oligomer identification has been performed using the protocols reported in  and . In detail, after 2 min of the substrate treatment, the liquors were removed and the oxidation was halted by the addition of
5 %w/waqueous solution of sodium dithionite and
acid-ified to pH 4 with 3 M HCl. The reaction mixture was extracted repeatedly with ethyl acetate (3 × 250 mL), and the combined organic layers were dried over sodium sul-fate and taken to dryness.
The residue was acetylated with acetic anhydride-pyridine 95:5 (v/v) and fractionated by preparative TLC
(CHCl3/MeOH 98:2) to identify the constituents by
comparison with synthetic standards with known structure.
The optical reflectivity measurements were performed on both empty and impregnated PSi matrices to explore the impregnation procedure. In Figure 4 we show optical reflectivity spectra obtained on two PSi samples, where the thin-layer Fabry-Pérot interference fringes are clearly Figure 3Schematic path of eumelanin formation  and
visible. The red curve corresponds to an impregnated PSi sample and the blue curve to an empty one with equal thickness. The discontinuity for wavelengths longer than 890 nm in the red curve is due to instrumental adjust-ment routine at the detector change. There are two main differences between the two curves. The first one is in the intensity of the interference fringes. The fact that the impregnated sample shows less intense fringes can be attributed to an increase of the absorption coefficient of the layer . The second difference between the two curves is the higher number of fringes per wavelength range for the impregnated sample. This increase can be correlated to an increase of the optical thickness of the sample . Given that the two samples have the same nominal thickness, this difference is clearly related mainly to the change in the refractive index.
In Figure 5 we show the dependence of the interference peak maxima number on the inverse of the wavelength for the two samples of Figure 4, the color code being also the same. If the refractive index had been constant, this plot would have been a straight line . In our case, however, considering the large spectral range explored, the refract-ive index is not constant. For this reason, the curves have been fitted separately for the higher (left) and lower (right) energy sides of the spectra. Since the slopes of the linear fits related to the impregnated sample are always higher than those related to the empty sample, the results of Figure 4 demonstrate that the refractive index of the impregnated PSi layer is higher than that of the empty PSi layer in the whole spectral range examined. From the results of Figures 4 and 5, we can then conclude that the eumelanin impregnation process leads to an increase of both the absorption coefficient and the refractive index of the PSi matrix. Moreover, the absence of beats in the interference fringes of the impregnated layer indicates that
the impregnation process is quite homogeneous through-out the whole PSi thickness and that there is no double layer given by a partial, depth-limited, eumelanin pore penetration.
These results are in agreement with the reported litera-ture absorption coefficients of eumelanin and PSi. To show this, in Figure 6, we plot the absorption coefficients of 78 % p+-type and 58 % p-type porous Si , bulk Si , and eumelanin . The absorption coefficients dispersion curves for eumelanin have been obtained from thin (80 nm) and thick (800 nm) film. All symbols are explained in the figure caption.
The data shown in Figure 6 clearly evidenced that the optical absorption coefficient of both thin and thick eumelanin films is significantly greater than that of PSi and even bulk silicon for photon energies lower than 2.5 eV (500 nm). For wavelengths longer than 600 to 650 nm, the eumelanin absorption coefficient is still sig-nificant (well above than 104cm−1) and more than a fac-tor of ten larger than that of PSi whose absolute value becomes less than 103 cm−1. This is where the effect of eumelanin may be expected to generate a more signifi-cant difference in the photoconductive behavior of empty and impregnated porous layers. It is important to note that from , the eumelanin absorption coefficient at 1,400 nm is still more than 6,000 cm−1 for thin films and 8,000 cm−1for thick films.
The photoconductive properties of porous Si samples were studied with and without eumelanin for unoxidized layers. A few samples were oxidized at several oxidation levels. This test has been done because, although the partial oxidation process may reduce the PSi conductiv-ity, the oxidation-induced modification of the eumelanin adhesion to the pore walls could, in principle, more than counterbalance the effect. In all cases, however, all the
Wavelength (nm) impregnated PSi
Effect of eumelanin impregnation on 5 m thick PSi
partially oxidized samples showed no measurable photo-sensitivity. Whatever the impinging light intensity value
(up to a maximum of about 200 W/m2) is, with and
without eumelanin, our results conclusively show that even a thin oxide layer on the pore's wall is sufficient to severely limit the layers' photosensitivity.
All non-oxidized samples, for all eumelanin im-mobilization approaches considered here, showed a marked photosensitivity. When illuminating with the whole lamp spectrum, the variation in the photocurrent intensity from very low ambient light to the maximum im-pinging light intensity showed an increase of more than
three orders of magnitude, fully reproducible for the same gold plot. However, while the wavelength dependence was highly reproducible, as discussed later in more detail, a variability was observed in the maximum measured photocurrent when using different gold contacts on the same sample and/or on different samples, even if nomin-ally identical. At the same time, the maximum photogen-erated voltage showed a much lower variation, being between 100 and 150 mV for impregnated samples and between 120 and 200 mV for empty samples, suggesting a contact-related and non material-related issue. Empty PSi layers showed more stable results with respect to the 25
Interfecerce fringes numbering (a.u.)
1/ peak (x10
Evolution of the interference fringes maxima as a function of 1/peak
eumelanin impregnated PSi empty PSi
Figure 5Interference peak ordinal vs. the inverse of the peak wavelength obtained from the data of Figure 4.Blue triangles refer to the empty PSi layer and red circles to the eumelanin-impregnated PSi layer. The linear fits of the experimental data are also shown for the lower (right) and higher (left) energy sides of the explored spectral range.
0 3 x cm -1 )
p+ PSi, 78% porosity p PSi, 58% porosity
eumelanin - thin layer eumelanin - thick layer
impregnated samples. The maximum absolute photocur-rent values measured with full illumination for impreg-nated and empty PSi were within about a factor of two, while the photovoltage measurement were much closer (5.1 mA/200 mV for empty PSi and 2.2 mA/150 mV for impregnated samples). The observed variability did not appear to depend on the eumelanin immobilization procedure.
To better evaluate the effect of the eumelanin insertion on the photoconductive properties of the samples and to discriminate possible contact issues from the samples' be-havior, we measured the wavelength dependence of the light response of impregnated and empty porous Si sam-ples using low-pass optical filters in front of the samsam-ples. By this approach, using a given filter the light arriving onto the samples' surface will only have wavelengths longer than the cutoff filter's. This means that the photocurrent measured with each filter will be given by all photocarriers generated by the interaction of the samples with the re-sidual spectral range, that is, the part whose photon en-ergy is lower than that characteristic of the cutoff filter. Consequently, if the carrier photogeneration occurs in the whole source spectrum, the plot of the photocurrent as a function of the cutoff wavelengths is expected to be a monotone curve which is increasing when moving to-wards shorter wavelengths. The results obtained on typical samples in our experiments are shown in Figure 7. The samples indicated as‘empty PSi 1’and‘impregnated PSi 1’ are the same samples whose optical reflectivity spectra have been shown in Figure 4. The absolute current values are comparable (Imax= 0.8μA for the two empty PSi layers
and Imax= 0.9 μA for the impregnated sample labeled
impregnated PSi 1) for three of the samples shown, while for one of the impregnated samples, the maximum abso-lute photocurrent is significantly lower (Imax= 0.09 μA,
Vmax= 100 mV with full spectral range illumination).
To separate the contact-related issues from the photoge-neration behavior of the samples, the photocurrent inten-sity and the wavelength dependent photogeneration behavior must be separated. If the behavior of the samples would prove to be the same with respect to the maximum recorded photocurrent, it would be possible to attribute the intensity differences from sample to sample essentially to contact-related issues and not to the hybrid material building procedure adopted. Accordingly, we show in Figure 8 the photocurrents of the two impregnated PSi samples of Figure 7, normalized by dividing each value by the maximum measured photocurrent of that sample. As in Figure 7, the normalized photocurrents are plotted vs. the low-pass filters cutoff wavelengths. Please note, however, that the peak at 500 nm of the impregnated PSi 1 sample, being clearly due to signal noise, has not been used as a reference for the normalization.
The striking feature of Figure 8 is the almost complete superposition of the two curves, indicating that the rela-tive behavior of the two impregnated samples is the same, despite the factor of 20 within their maximum values. This clearly indicates, as stated above, that the observed photocurrent intensity fluctuation is funda-mentally related to the contact fabrication process and does not point to a poor reproducibility of the hybrid material behavior.
From the results shown in Figures 7 and 8, there are several considerations that can be made. First, all curves
Filters cutoff wavelengths (nm) impregnated PSi 1
impregnated PSi 2 empty PSi 1 empty PSi 2
Photocurrent of impregnated and empty PSi matrices as a function of the
show a monotonic photocurrent increase when going from longer to shorter wavelengths, indicating that the ab-sorption takes place in the whole available light spectrum for both impregnated and empty PSi layers. The second significant feature is that impregnated samples show a steep photocurrent increase in the lower energy part of the spectrum. This is coherent with what can be expected by the comparison of the optical absorption coefficients of the materials, as discussed earlier in this work. If we com-pare empty and impregnated samples with similar max-imum photocurrent, about 40 % of the total photocurrent is generated, for impregnated samples, when using wave-lengths longer than 780 nm; while for empty PSi layers, the same wavelength range gives only about 15 % of the maximum photocurrent.
The latter effect is even more significant if we keep in mind the very low intensity of the impinging light in the 700 to 850 nm range: for the impregnated samples, 40 % of the total photocurrent is obtained with a very limited part of the total spectrum; while to obtain the same amount of photocurrent with the empty PSi samples, we need to increase the wavelength range up to 550 nm, in-cluding most of the available lamp spectral range.
These results show how the impregnation of the PSi matrix with eumelanin significantly increases the capabil-ity of the layer to efficiently photogenerate carriers from light especially when approaching the infrared region.
We have shown that the photovoltaic properties of PSi may be significantly improved by impregnation with eumelanin. In particular, we showed that introducing the pigment in the porous Si matrix leads to a significantly
more efficient photocurrent generation in the lower en-ergy part of the experimental wavelength range explored with respect to empty porous Si layers.
This result not only contributes to expand the scope of heterojunctions in developing a new hybrid material but also provides the first evidence of the eumelanin capability to efficiently collect the photon energy. In a given substrate, eumelanin seems to act as a kind of ‘
an-tenna’, modifying the range of the useful wavelength
range for photoconversion application.
Although further experimental and theoretical studies are needed to improve the electrical contacts reproducibil-ity and to reach a deeper understanding of the observed behavior in view of future development and applications, the proof of principle device presented here opens a new window into the evolving panorama of eumelanin-based devices and contributes to the development of bioinspired and biocompatible optoelectronic devices.
The authors declare that they have no competing interests.
One of the authors (AP) acknowledges partial financial support by Ministry of Education, Universities and Research (MIUR, Italy), PRIN 2008 project. Andrea Falqui from the Italian Institute of Technology, Genova, Italy is gratefully acknowledged for the SEM measurements.
Author details 1
Dipartimento di Fisica, Cittadella Universitaria di Monserrato, Università degli Studi di Cagliari, S.P. 8 km 0.7, Monserrato (Ca) 09042, Italy.2Dipartimento di
Scienze Chimiche, Università degli Studi di Napoli Federico II, Complesso Universitario di Monte Sant'Angelo, Via Cintia, Napoli 4-80126, Italy.
GM conceived of the study, participated in its design and coordination, prepared part of the samples and performed the reflectivity measurements and analysis. LM performed the photoconductivity measurements and
Cutoff wavelength (nm) Normalized photocurrents
for the PSi samples of Figure 5
impregnated PSi 1 impregnated PSi 2
prepared part of the samples. SS participated in the design of the study. AP participated in the design of the study, carried out the eumelanin
preparation and performed the PSi impregnation process with eumelanin. All authors contributed to the data analysis. All authors read and approved the final manuscript.
Received: 23 April 2012 Accepted: 9 July 2012 Published: 9 July 2012
1. Kippelen B, Brédas J-L:Organic photovoltaics.Energ Environ Sci2009,2:251. 2. Nguyen T-P:Polymer-based nanocomposites for organic optoelectronic
devices.A review. Surf Coat Tech2011,206:742–752.
3. Günes S, Sariciftci NS: Hybrid solar cells.Inorg Chim Acta2008,
4. Lee J, Jho JY:Fabrication of highly ordered and vertically oriented TiO2
nanotube arrays for ordered heterojunction polymer/inorganic hybrid
solar cell.Sol Energ Mat Sol C2011,95:3152–3156.
5. Yu G, Gao J, Hummelen JC, Wudl F, Heeger AJ:Polymer photovoltaic cells: enhanced efficiencies via a network of internal donor-acceptor
6. Arici E, Meissner D, Schaffler F, Sariciftci NS:Core/shell nanomaterials in
photovoltaics.Int J Photoenergy2003,5:199–208.
7. Sanchez C, Julián B, Belleville P, Popall M:Applications of hybrid organic–
inorganic nanocomposites.J Mater Chem2005,15:3559–3592.
8. Saunders BR, Turner ML:Nanoparticle-polymer photovoltaic cells.Adv Colloid Interfac2008,138:1–23.
9. Wang TH, Iwaniczko E, Page MR, Levi DH, Yan Y, Yelundur V, Branz HM, Rohatgi A, Wang Q:Effective interfaces in silicon heterojunction solar cells. Lake Buena Vista, Florida (USA): 31st IEEE Photovoltaic Specialists Conference and Exhibition, January 3-7, 2005; 2005:955–958. doi:DOI 10.1109/ PVSC.2005.1488290.
10. Wang Q, Page MR, Iwaniczko E, Xu Y, Roybal L, Bauer R, To B, Yuan H-C, Duda A, Hasoon F, Yan YF, Levi D, Meier D, Branz HM, Wang TH:Efficient
heterojunction solar cells onp-type crystal silicon wafers.Appl Phys Lett
11. Hoppe H, Sariciftci NS:Organic solar cells: an overview.J Mater Res2011, 19:1924–1945.
12. Nelson J:Organic photovoltaic films.Curr Opin Solid St M2002,6:87–95. 13. Halls JJM, Walsh CA, Greenham NC, Marseglia EA, Friend RH, Moratti SC,
Holmes AB:Efficient photodiodes from interpenetrating polymer
14. Yoshino K, Tada K, Fujii A, Conwell EM, Zakhidov AA:Novel photovoltaic devices based on donor-acceptor molecular and conducting polymer
systems.IEEE T Electron Dev1997,44:1315–1324.
15. Yu G, Heeger AJ:Charge separation and photovoltaic conversion in polymer composites with internal donor / acceptor heterojunctions. J Appl Phys1995,78:4510–4515.
16. Abbas M, D’Amico F, Morresi L, Pinto N, Ficcadenti M, Natali R, Ottaviano L, Passacantando M, Cuccioloni M, Angeletti M, Gunnella R:Structural,
electrical, electronic and optical properties of melanin films.Eur Phys J E
17. Jastrzebska M, Kocot A, Vij JK, Zalewska-Rejdak J, Witecki T:Dielectric
studies on charge hopping in melanin polymer.J Mol Struct2002,
18. Meredith P, Sarna T:The physical and chemical properties of eumelanin. Pigm Cell Res2006,19:572–594.
19. Salis A, Setzu S, Monduzzi M, Mula G:Porous silicon-based electrochemical
biosensors. InBiosensors - Emerging Materials and Applications. Edited by
Serra PA.: INTECH; 2011:333–352. http://www.intechopen.com/books/ biosensors-emerging-materials-and-applications/porous-silicon-based-electrochemical-biosensors.
20. Anglin EJ, Cheng L, Freeman WR, Sailor MJ:Porous silicon in drug delivery
devices and materials.Adv Drug Deliver Rev2008,60:1266–1277.
21. Chan S, Fauchet PM:Tunable, narrow, and directional luminescence from
porous silicon light emitting devices.Appl Phys Lett1999,75:274–276.
22. Badawy WA:Effect of porous silicon layer on the performance of Si/
oxide photovoltaic and photoelectrochemical cells.J Alloy Compd2008,
23. Vernon SM, Kalkhoran NM, Maruska HP, Halverson WD:High performance
porous silicon solar cell development.Proceedings of 1994 IEEE 1st World
Conference on Photovoltaic Energy Conversion - WCPEC, IEEE1994,2:1583– 1586.
24. Ünal B, Parbukov AN, Bayliss SC:Photovoltaic properties of a novel stain
etched porous silicon and its application in photosensitive devices.Opt
25. Nahor A, Berger O, Bardavid Y, Toker G, Tamar Y, Reiss L, Asscher M, Yitzchaick S, Sa’ar A, Yitzchaik S:Hybrid structure of porous silicon and
conjugated polymers for photovoltaic applications.Phys Stat Sol2011,
26. Chao C-H, Chan C-H, Wu F-C, Huang J-J, Yang Lien S, Weng K-W, Cheng H-L: Efficient hybrid organic/inorganic photovoltaic cells utilizing n-type
pentacene and intrinsic/p-type hydrogenated amorphous silicon.Sol
Energ Mat Sol C2011,95:2407–2411.
27. Mayer T, Weiler U, Kelting C, Schlettwein D, Makarov S, Wohrle D, Abdallah O, Kunst M, Jaegermann W:Silicon–organic pigment material hybrids for
photovoltaic application.Sol Energ Mat Sol C2007,91:1873–1886.
28. Zubov VP, Ishchenko AA, Storozhenko PA, Bakeeva IV, Kirilina YO, Fetisov GV:
Organic–inorganic hybrid hydrogels containing nanocrystalline silicon.
29. Prota G:Melanins and Melanogenesis. San Diego: Academic Press; 1992. 30. D’Ischia M, Napolitano A, Pezzella A, Meredith P, Sarna T:Chemical and
structural diversity in eumelanins: unexplored bio-optoelectronic
materials.Angew Chem Int Edit2009,48:3914–3921.
31. Meredith P, Powell BJ, Riesz J, Nighswander-Rempel SP, Pederson MR, Moore EG:Towards structure–property–function relationships for
32. D'Ischia M, Napolitano A, Pezzella A:5,6-Dihydroxyindole chemistry:
unexplored opportunities beyond eumelanin.Eur J Org Chem2011,
33. Subianto S, Will G, Meredith P:Processes for the production of thin films of melanin and melanin- like molecules.International Patents Application2004, PCT/AU20047001244.
34. Rosei MA, Mosca L, Galluzzi F:Photoelectronic properties of synthetic
35. Bloisi F, Pezzella A, Barra M, Chiarella F, Cassinese A, Vicari L:Matrix assisted
pulsed laser deposition of melanin thin films.J Appl Phys2011,
36. Bloisi F, Pezzella A, Barra M, Alfè M, Chiarella F, Cassinese A, Vicari L:Effect of substrate temperature on MAPLE deposition of synthetic eumelanin
films.Appl Phys A: Mater2011,105:619–627.
37. Setzu S, Salis S, Demontis V, Salis A, Monduzzi M, Mula G:Porous
silicon-based potentiometric biosensor for triglycerides.Phys Stat Sol (a)2007,
38. Sailor MJ:Porous Silicon in Practice: Preparation. Weinheim: Wiley-VCH; 2012. 39. Salis A, Cugia F, Setzu S, Mula G, Monduzzi M:Effect of oxidation level
ofn+-type mesoporous silicon surface on the adsorption and the
catalytic activity ofCandida rugosalipase.J Colloid Interf Sci2010,
40. Pezzella A, Iadonisi A, Valerio S, Panzella L, Napolitano A, Adinolfi M, d’Ischia
M:Disentangling eumelanin“black chromophore”: visible absorption
changes as signatures of oxidation state- and aggregation-dependent dynamic interactions in a model water-soluble
5,6-dihydroxyindole polymer.J Am Chem Soc2009,131:15270–15275.
41. Edge R, D’Ischia M, Land EJ, Napolitano A, Navaratnam S, Panzella L, Pezzella A, Ramsden CA, Riley PA:Dopaquinone redox exchange with
dihydroxyindole and dihydroxyindole carboxylic acid.Pigm Cell Res2006,
42. Napolitano A, Pezzella A, D’Ischia M, Prota G:New pyrrole acids by oxidative degradation of eumelanins with hydrogen peroxide further
hints to the mechanism of pigment breakdown.Tetrahedron1996,
43. Pezzella A, Ambrogi V, Arzillo M, Napolitano A, Carfagna C, d’Ischia M: 5,6-Dihydroxyindole oxidation in phosphate buffer/polyvinyl alcohol: a new model system for studies of visible chromophore development
in synthetic eumelanin polymers.Photochem Photobiol2008,
45. Pacholski C, Sartor M, Sailor MJ, Cunin F, Miskelly GM: Biosensing using porous silicon double-layer interferometers: reflective
interferometric Fourier transform spectroscopy. J Am Chem Soc 2005,
46. Green MA:Self-consistent optical parameters of intrinsic silicon at
300 K including temperature coefficients.Sol Energ Mat Sol C2008,
Cite this article as:Mulaet al.:Photovoltaic properties of PSi impregnated with eumelanin.Nanoscale Research Letters20127:377.
Submit your manuscript to a
journal and beneﬁ t from:
7Convenient online submission
7Rigorous peer review
7Immediate publication on acceptance
7Open access: articles freely available online
7High visibility within the ﬁ eld
7Retaining the copyright to your article